Ó Operative Dentistry, 2012, 37-2, 000-000 Degree of Conversion of Simplified Contemporary Adhesive Systems as Influenced by Extended Air-Activated or Passive Solvent Volatilization Modes BCD Borges EJ Souza-Junior WC Brandt AD Loguercio MAJR Montes RM Puppin-Rontani MAC Sinhoreti Clinical Relevance Active air-drying for 60 seconds to volatilize solvents can be necessary to increase the degree of conversion of some adhesive systems, which might be related to improved clinical performance.Boniek C. D. Borges, DDS, MSc, Potiguar University SUMMARY (Laureate International Universities), Department of Den- This study evaluated the effect of five methods tistry, Natal, Brazil of solvent volatilization on the degree of con-*Eduardo Jose Souza-Junior, DDS, MS, PhD student, Piraci- version (DC) of nine one-bottle adhesive sys- caba Dental School, State University of Campinas–UNI- tems using Fourier transform infrared/ ˜ CAMP, Restorative Dentistry, Sao Paulo, Brazil attenuated total reflectance (FTIR/ATR) anal-William C. Brandt, PhD, University of Taubate, Department ysis. Nine adhesives were tested: Adper Single ˜ of Prosthodontics, Sao Paulo, Brazil Mario Alexandre Coelho Sinhoreti, DDS, MSc, PhD, Piracica-Alessandro D. Loguercio, DDS, PhD, MSc, University Estad- ba Dental School, University of Campinas, Restorative ual de Ponta Grossa, Restorative Dentistry, Ponta Grossa, ˜ Dentistry, Sao Paulo, Brazil Brazil *Corresponding author: Piracicaba Dental School, StateMarcos A. J. R. Montes, DDS, MSc, PhD, University of University of Campinas–UNICAMP, Restorative Dentist- Pernambuco, Departament of Restorative Dentistry, Per- ˜ ˜ ry, Av. Limeira, 901, Areiao, PO Box 52, Piracicaba, Sao nambuco, Brazil Paulo 13414-903, Brazil; e-mail: firstname.lastname@example.orgRegina M. Puppin-Rontani, DDS, MSc, PhD, Piracicaba DOI: 10.2341/11-248-L ˜ Dental School, Pediatric Dentistry, Sao Paulo, Brazil
2 Operative DentistryBond 2 (SB), Adper Easy One (EO), One Up the way the acidic primer and bonding resin areBond F Plus (OUP), One Coat Bond SL (OC), XP provided by the manufacturer.2 An immediateBond (XP), Ambar (AM), Natural Bond (NB), consequence of adhesive simplification is sacrificeGO, and Stae. The adhesive systems were of the universality of multistep adhesives,3 andapplied to a zinc-selenide pellet and 1) cured simplified systems are currently preferred by clini-without solvent volatilization, 2) left undis- cians to perform adhesive procedures because of timeturbed for 10 seconds before curing, 3) left savings.undisturbed for 60 seconds before curing, 4) Successful adhesion to hard tissues is a funda-air-dried with an air stream for 10 seconds mental requirement prior to the placement of dentalbefore curing, and 5) air-dried with an air materials and is directly dependent on the quality ofstream for 60 seconds before curing. FTIR/ATR the hybrid layer. Hence, any approach to prolong thespectra were obtained, and the DC was calcu- lifetime of adhesives might focus on improving thelated by comparing the aliphatic bonds/refer- stability of the bonding interface of these biomate-ence peaks before and after light activation for rials to tooth tissues.4 Optimal monomer infiltration10 seconds (FlashLite 1401). The DC means of into the demineralized substrates and the achieve-each material were analyzed by one-way anal- ment of a high degree of conversion (DC) are crucialysis of variance and post hoc Tukey test factors in establishing long-lasting bonds.5 A low DC(p,0.05). The DC of GO and Stae adhesive of dental adhesives is associated with low bondsystems was not affected by the five evapora- strength values and mechanical properties, hightion conditions. Air-drying for 60 seconds be- monomer elution, increased permeability, and phasefore curing yielded the highest DC for SB, EO, separation.6-8 Moreover, reduced DC even accountsand OC. Extended solvent volatilization time for the possible continuous etching of the tooth(60 seconds) either with or without air-drying substrate due to suboptimally polymerized acidicbefore curing provided the highest DC for AM, monomer in self-etch adhesives.9 Thus, obtaining aNB, XP, and OUP. Thus, the monomer conver- high DC of adhesive systems is a crucial factor in thesion of adhesive systems was material depen- long-term stability of the hybrid layer.dent. In general, the 60-second passive oractive air-drying modes to volatilize solvents Simplified dental bonding agents are composed ofbefore curing enhanced the degree of conver- a mixture of hydrophilic primers and hydrophobicsion for the one-bottle simplified adhesive adhesive resins dissolved in acetone, ethanol, water,systems. or some combination of the solvents, which play an important role in the bond performance.10 Although INTRODUCTION the presence of solvents makes the process of monomer infiltration easier, the remaining waterThe development of adhesive systems has completely and organic solvents can greatly inhibit the poly-changed the traditional concepts of dentistry. Today, merization reaction and compromise the creation of aadhesive systems are widely used in direct proce- well-defined polymer matrix.11 The use of air spraydures for restoration of anterior and posterior to accelerate solvent evaporation has been recom-cavities, fissure sealing, reattachment of fractured mended by the manufacturers, and several tech-fragments, and corrections in tooth morphology and niques have been evaluated by researchers. It hasin indirect procedures involving cementation of root- been shown that the extended passive solventcanal posts and indirect ceramic and composite volatilization that occurs when adhesive systemscrowns.1 are left undisturbed for 60 seconds with or without Based on the management of the smear layer posterior air-drying for 10 seconds before photo-substrate, contemporary adhesive systems are cate- activation may increase the DC of some commercial-gorized as etch-and-rinse (ER) and self-etch (SE) ly available adhesive systems.12 However, little issystems. Both bonding strategies are also available known about the DC of contemporary adhesivein a full or simplified version. When the conditioning systems with respect to whether an extended air-step is followed by a priming step and application of activated drying mode to volatilize the solventthe adhesive resin, ER adhesives are available in should be performed before curing. Thus, this studythree steps, or they are available in a two-step aimed to evaluate the DC of commercially availableprocedure when the primer and adhesive resin are adhesive systems when photo-activated after ex-joined into one application. Similarly, SE adhesives tended air-activated or passive methods of solventcan employ two steps or a single one, depending on volatilization. The null hypothesis was that there is
Borges Others: Degree of Conversion of Adhesive Systems 3no difference in the DC of adhesive systems when based adhesive), the intensity of the carbonylphoto-activated after different conditions of solvent reference peak (located at 1716 cmÀ1) was obtained.evaporation. The DC (%) was calculated using the following equation: DC (%) = 100 3 [1 À (R polymerized/R MATERIALS AND METHODS nonpolymerized)], where R represents the ratioExperimental Design between the absorbance peak at 1638 cmÀ1 and 1608 cmÀ1 (for SB, EO, OC, OUP, AM, and XP), 1638Nine one-bottle commercially available adhesive cmÀ1 and 1537 cmÀ1 (for GO and Stae), and 1638systems with different solvents were tested: Adper cmÀ1 and 1716 cmÀ1 (for NB).Single Bond 2 (SB; 3M ESPE, St Paul, MN, USA),Adper Easy One (EO; 3M ESPE), One Up Bond F The data were analyzed by one-way analysis ofPlus (OUP; Tokuyama, Tokyo, Japan), One Coat variance and post hoc Tukey test (only an intrabrand ` ¨Bond SL (OC; Coltene/Whaledent, Altsatten, Swit- comparison was performed to compare the differencezerland), XP Bond (XP; Dentsply/Caulk, Milford, DE, among the tested solvent volatilization modes forUSA), Ambar (AM; FGM, Joinville, SC, Brazil), each adhesive resin). Statistical significance wasNatural Bond (NB; DFL, Rio de Janeiro, RJ, Brazil), established at a=0.05.GO (SDI, Victoria, Australia), and Stae (SDI).Moreover, five modes of solvent volatilization were RESULTSperformed before curing: 1) immediate cure without The means and standard deviations of the degree ofsolvent volatilization, 2) passive solvent volatiliza- conversion values are presented in Table 2. Only thetion (left undisturbed) for 10 seconds, 3) passive application of air for 60 seconds yielded a statisti-solvent volatilization for 60 seconds (left undis- cally higher degree of conversion for SB, EO, andturbed), 4) active solvent volatilization for 10 seconds OC. Both extended times of solvent volatilization (60(with air stream), and 5) active solvent volatilization seconds; active and passive methods) promotedfor 60 seconds (with air stream). The composition, statistically increased monomer conversion for AM,classification, manufacturers, and lot number of all NB, XP, and OUP. On the other hand, the degree ofadhesives systems tested are displayed in Table 1. conversion of GO and Stae was not influenced by the volatilization technique.DC AnalysisThe DC was analyzed by Fourier transform infrared/ DISCUSSIONattenuated total reflectance (Spectrum 100, Perki- The null hypothesis tested in this study was rejectednElmer, Shelton, XX, USA) at 248C under 64% because the degree of conversion of most adhesivesrelative humidity. One drop of each adhesive system was affected by different solvent volatilization(n=5) was applied to the surface of a zinc selenide methods. Air volatilization for 60 seconds providedpellet (PerkinElmer). Before curing for 10 seconds the statistically highest monomer conversion for twowith an LED light (FlashLite 1401, Discus Dental, ethanol-based (SB and EO) and one water-basedCulver City, CA, USA; irradiance at 1100 mW/cm2) (OC) adhesive system tested, whereas either air orpositioned 3 mm from the pellet surface, the solvent passive volatilization methods for 60 seconds yieldedof each adhesive resin was volatilized in accordance the highest monomer conversion for other ethanol-with the aforementioned modes. based (AM, NB) and water-based (OUP) adhesive The absorption spectra of nonpolymerized and systems and for the tertiary-alcohol-based (XP)polymerized adhesive resins were obtained from the adhesive system. Nevertheless, none of the testedregion between 4000 and 650 cmÀ1 with 32 scans at 4 solvent volatilization techniques affected the mono-cmÀ1. For adhesive systems containing aromatic mer conversion of the acetone-based adhesive sys-vinyl bonds of bisphenol and aliphatic bonds of the tems evaluated in the present investigation.methacrylate functional group (SB, EO, OC, OUP, Solvent volatilization can facilitate the polymeri-AM, XP), the aliphatic carbon-to-carbon double-bond zation reaction because the distance among mono-absorbance peak intensity (located at 1638 cmÀ1) and mers is reduced, increasing the degree ofthat of the aromatic component (located at 1608 conversion.13 Ideally, solvents should be completelycmÀ1; reference peak) were obtained. For Stae and volatilized from the applied mixture prior to poly-GO, which do not present aromatic dimethacrylates, merization. However, it has been shown thatthe intensity of the urethane reference peak (located solvents cannot be completely removed from adhe-at 1538 cmÀ1) was obtained. For NB (a TEGDMA- sive systems.14 As water/solvent volatilizes from the
4 Operative DentistryTable 1: Composition, Manufacturer, and Lots of the Adhesive Systems Used in This Study Adhesive Systems Composition (% by Weight) Classification Manufacturer Lot No.Adper Single Bond 2 Ethyl alcohol (25–30), silane treated silica Two-step ER 3M ESPE, St Paul, MN, USA 8PT (nanofiller) (10–20), Bis-GMA (10–20), HEMA (5-10), glycerol 1,3-dimethacrylate (5-10), copolymer of acrylic and itaconic acids (5-10), water (,5), diurethane dimethacrylate (1–5)Adper Easy One Bis-GMA (15–25), HEMA (15–25), ethanol One-step SE 3M ESPE, St Paul, MN, USA 84020 (10–15), water (10–15), phosphoric acid-6- methacryloxy-hexylesters (5-15), silane treated silica (8-12), 1,6-hexanediol dimethacrylate (5- 10), copolymer of acrylic and itaconic acid (1– 5), (dimethylamino)ethyl methacrylate (1–5), camphorquinone (1–3), 2,4,6- trimethylbenzoyldiphenylphosphine oxide (1–3)One Up Bond F Plus Agent A: Methacryloyloxyalkyl acid phosphate One-step SE Tukoyama, Tokyo, Japan 61184 (30–60), MAC-10 (10–30), methyl methacrylate (10–20), Bisphenol A polyethoxy methacrylate (20–40) Agent B: HEMA (30–60), methyl methacrylate (10–30), fluoroaminosilicate glass filler (10–15), borate catalyst (,5), purified water (5-20)One Coat Bond SL Methacrylate (a), polyalkenoat methacryliert (a), Two-step ER ` ¨ Coltene/Whaledent, Altsatten, 0173809 water (a) SwiterlandXP Bond Methacrylates (25–50), tert-butyl alcohol (10– Two-step ER Dentsply/Caulk, Milford, DE, USA 17056CB 25), acrylates (10–25)Ambar UDMA (5-40), HEMA (5-40), methacrylate Two-step ER FGM, Joinville, SC, Brazil 161210 acidic monomers (1–20), methacrylate hydrophilic monomers (5-40), silanized silicon dioxide (,1), camphorquinone (,1), 4-EDAMB (,1), ethanol (,20)Natural Bond PMGDM (a), TEGDMA (a), HEMA (a), PHFA Two-step ER DFL, Rio de Janeiro, RJ, Brazil 10121648 (a), camphorquinone (a), 4-EDAMB (a), butyl- hydroxytoluene (a), ethanol (a)GO Acetone (30–50), acrylic monomer (30–50), One-step SE SDI, Victoria, Australia 164413 balance ingredient (non-hazardous) (10–15)Stae Acetone (54), acrylic monomer (44), balance Two-step ER SDI, Victoria, Australia 090301 ingredient (non-hazardous) (2)Abbreviations: Bis-GMA, bisphenol A-glycidyl methacrylate; ER, etch-and-rinse; EDAMB, ethyl 4-dimethylaminobenzoate; HEMA, 2-hydroxyethyl methacrylate;MAC-10, 11-methacryloxy-1,1-undecanedicarboxylic acid; PHFA, potassium hexafluoroantimonate; PMGDM, pyromellitic glycerol dimethacrylate; SE, self-etching;TEGDMA, triethyleneglycol dimethacrylate; UDMA, urethane dimethacrylate.a Not provided by the manufacturer.
Borges Others: Degree of Conversion of Adhesive Systems 5 Table 2: Degree of Conversion Means (Standard Deviations) of Adhesive Systems According to Volatilization Conditions of Solventsa Adhesive Systems Immediate 10-Second Passive 60-Second Passive 10-Second Active 60-Second ActiveAdper Single Bond 2 75.5 (0.3) C 75.0 (0.6) C 77.4 (0.7) B 77.1 (0.7 ) B 79.7 (0.2) AAdper Easy One 48.9 (0.4) B 48.9 (0.2) B 49.6 (0.4) B 50.8 (0.1) B 55.5 (1.5) AOne Up Bond F Plus 89.9 (0.5) B 89.5 (0.7) B 94.6 (0.4) A 90.4 (0.3) B 95.7 (0.2) AOne Coat Bond SL 77.5 (0.3) C 78.5 (0.5) BC 80.1 (1.0) AB 79.5 (0.4) BC 82.2 (0.9) AXP Bond 52.4 (0.3) B 58.1 (0.7) B 67.4 (0.8) A 66.0 (0.5) AB 68.8 (0.1) AAmbar 39.8 (1.7) C 44.1 (2.0) BC 57.6 (4.8) A 50.4 (2.2) AB 58.2 (3.0) ANatural Bond 24.3 (2.0) C 28.9 (3.8) C 51.6 (1.2) A 42.6 (2.5) B 50.8 (0.6) AGO 82.9 (0.5) A 82.6 (0.6) A 83.7 (0.2) A 82.6 (0.8) A 83.9 (0.3) AStae 80.8 (0.1) A 80.8 (0.1) A 75.6 (0.9) A 79.1 (0.1) A 79.0 (0.4) A a Means followed by different capital letters differ statistically by Tukey test (p 0.05). No comparison among the products was performed.adhesive, monomer density is found to increase solvent.17 The higher the formation of hydrogensharply, creating a monomer concentration gradient bonds is between solvent and monomers, the morethat acts as a barrier for further solvent evaporation, difficulty there will be in volatilizing the solvent.reducing the ability of water and solvents to Although the solvent type is an essential factor,volatilize from the adhesive.15 Thus, clinicians other ingredients in adhesive systems can influenceshould attempt to remove the highest amount of solvent volatilization and, consequently, the mono-solvent to achieve an adequate monomer conversion. mer conversion. For these reasons, the differentIn fact, a low DC of adhesive systems is associated solvent volatilization methods provided statisticallywith low bond strength values and mechanical different degrees of conversion means for ethanol-properties, high monomer elution, increased perme- and water-based adhesive systems with similarability, and phase separation.6-8 Moreover, reduced solvents but differing in their chemical components.DC even accounts for the possible continuous etching For SB and EO, it is likely that a greater formationof the tooth substrate due to suboptimally polymer- of hydrogen bonds was achieved so that only activeized acidic monomer in self-etch adhesives.9 air to evaporate the solvent would be sufficient to Several factors have been related to the solvent break them, increasing solvent volatilization andretention in adhesive systems. Solvents with rela- monomer conversion. This might have not occurredtively low vapor pressure, such as water, when for AM, NB, and XP. For these materials, the degreemixed with nonvolatile monomers, become less able of conversion of the samples whose solvent wasto volatilize as monomer concentration increases.14 volatilized using either active air for 60 seconds or noOn the other hand, acetone, with a relatively high air application for 60 seconds was similar. Thus,vapor pressure of 184 mm Hg at 208C, volatilizes even in the absence of active air, an extended passivemuch faster than ethanol or water, with vapor method was probably enough to break the hydrogenpressure of 43.9 and 17.5 mm Hg, respectively.16 bonds, increasing the solvent volatilization andAlso, the extent of solvent retention in polymer degree of conversion means. This assumption alsonetworks depends on the resin polarity. The resin might be attributed to the water-based adhesivepolarity influences the number of hydrogen bonding systems tested. While OC obtained the highestsites and the attraction between the polymer and monomer conversion after only 60 seconds of air
6 Operative Dentistryapplication, OUP already had the highest monomer REFERENCESconversion means after the extended passive method 1. Reis A, Zander-Grande C, Kossatz S, Stanislawczuk R,to volatilize the solvent. Although further chemical Manso A, de Carvalho RM Loguercio AD (2010) Effectanalyses are necessary to confirm the aforemen- of mode of application on the microtensile bond strengthtioned assumptions, the reported results justify the of a self-etch and etch-and-rinse adhesive system Opera- tive Dentistry 35(4) 428-435.need to evaluate several commercially availableadhesive systems in different conditions of solvent 2. Breschi L, Mazzoni A, Ruggeri A, Cadenaro M, Di Lenarda R, De Stefano Dorigo E (2008) Dental adhesionvolatilization. review: aging and stability of the bonded interface Dental Both the acetone-based adhesive systems tested in Materials 24(1) 90-101.this study (GO and Stae) presented similar compo- 3. King NM, Tay FR, Pashley DH, Hashimoto M, Ito S,sition, although the components were in different ´ Brackett WW, Garcıa-Godoy F, Sunico M (2005)proportions. In addition to the high vapor pressure of Conversion of one-step to two-step self-etch adhesives for improved efficacy and extended application Americanacetone, its solubility for hydrogen bonding forces is Journal of Dentistry 18(2) 126-134.7 (J/cm3)1/2, compared with ethanol, for which it is 20 ´ 4. Reis A, Klein-Junior CA, de Souza FH, Stanislawczuk R,(J/cm3)1/2.18 That is, the affinity of the carbonyl Loguercio AD (2010) The use of warm air stream forgroup of acetone to the hydrogen bond with itself or solvent evaporation: effects on the durability of resin-water or any functional group on monomers that are dentin bonds Operative Dentistry 35(1) 29-36.capable of hydrogen bond formation is only about 5. Reis AF, Arrais CA, Novaes PD, Carvalho RM, De Goesone-third that of ethanol. This is why acetone is so MF, Giannini M. Ultramorphological analysis of resin-volatile.17 Thus, it is likely that the solvent might dentin interfaces produced with water-based single-stephave been volatilized during the adhesive photo- and two-step adhesives: nanoleakage expression Journalactivation, even without using a solvent volatiliza- Biomedical Materials Research. Part B, Applied Bioma- terials 71(1) 90-98.tion technique. Moreover, the heat generated fromthe curing light also might have facilitated acetone 6. Kanehira M, Finger WJ, Hoffmann M, Endo T, Komatsu M (2006) Relationship between degree ofvolatilization, yielding statistically similar degrees polymerization and enamel bonding strength with self-of conversion for the samples tested in this study. On etching adhesives Journal of Adhesive Dentistry 8(4)the other hand, it should be taken into account that 211-216.no residual moisture from the wet bonding technique 7. Wang Y, Spencer P, Yao X, Ye Q (2006) Effect ofwas mixed with adhesive solutions, which could coinitiator and water on the photoreactivity and photo-completely alter the solvent retention and monomer polymerization of HEMA/camphorquinone-based reactantconversion.13,19 Thus, clinicians should be encour- mixtures Journal of Biomedical Materials Research. Part A 78(4) 721-728.aged to volatilize the solvent even when using anacetone-based adhesive system, in particular by 8. Cadenaro M, Antoniolli F, Codan B, Agee K, Tay FR, Dorigo Ede S, Pashley DH, Breschi L (2010) Influenceusing more extended times than those recommended of different initiators on the degree of conversion ofby the manufacturers. experimental adhesive blends in relation to their hydro- philicity and solvent content Dental Materials 26(4) CONCLUSION 288-294.Therefore, the degree of conversion of the adhesive 9. Wang Y, Spencer P (2005) Continuing etching of an all- in-one adhesive in wet dentin tubules Journal of Dentalsystems tested was material dependent. The etha- Research 84(4) 350-354.nol- and water-based adhesive systems tested bene- 10. Loguercio AD, Loeblein F, Cherobin T, Ogliari F, Piva E,fited from extended solvent volatilization time either Reis A (2009) Effect of solvent removal on adhesivewith or without air application. The acetone-based properties of simplified etch-and-rinse systems and onadhesive systems tested were not influenced by bond strengths to dry and wet dentin Journal of Adhesivesolvent volatilization techniques. Dentistry 11(3) 213-219. 11. Reis AF, Oliveira MT, Giannini M, de Goes MF, Acknowledgments Rueggeberg FA (2003) The effect of organic solvents on one-bottle adhesives’ bond strength to enamel and dentinThis study was partially supported by FAPESP (grant 07/ Operative Dentistry 28(6) 700-706.02800–3). The authors thank Vigodent (Rio de Janeiro, RJ,Brazil), FGM (Joinville, SC, Brazil), DFL (Rio de Janeiro, RJ, 12. Giannini M, Arrais CA, Vermelho PM, Reis RS, dosBrazil), and SDI (Victoria, Australia) for supporting material Santos LP, Leite ER (2008) Effects of the solventused in this investigation. evaporation technique on the degree of conversion of one- bottle adhesive systems Operative Dentistry 33(2)(Accepted 8 September 2011) 149-154.
Borges Others: Degree of Conversion of Adhesive Systems 713. Nunes TG, Garcia FCP, Osorio R, Carvalho RM, 16. Lide RR (ed) (1993) CRC Handbook of Chemistry and Toledano M (2006) Polymerization efficacy of simplified Physics Chemical Rubber Co, Cleveland, OH 6-169. adhesive systems studied by NMR and MRI techniques 17. Yiu CK, Pashley EL, Hiraishi N, King NM, Goracci C, Dental Materials 22(10) 963-972. Ferrari M, Carvalho RM, Pashley DH, Tay FR (2005) Solvent and water retention in dental adhesive blends14. Cadenaro M, Breschi L, Rueggeberg FA, Suchko M, after evaporation. Biomaterials 26(34) 6863-6872. Grodin E, Agee K, Di Lenarda R, Tay FR, Pashley DH (2009) Effects of residual ethanol on the rate and degree 18. Burke J. (1984) Solubility parameters: theory and applica- of conversion of five experimental resins Dental Materials tion In: Jensen C (ed) AIC Book and Paper Group Annual AIC Book and Paper Group, Washington, DC 13-58. 25(5) 621-628. 19. Garcia G, Fernandes KB, Garcia FC, D’Alpino PH, da15. Duskova-Smrkova M, Dusek K (2002) Processes and Rocha Svizero N, Wang L (2010) Solvent retention of states during polymer film formation by simultaneous contemporary commercial dentin bonding agents in a crosslinking and solvent evaporation Journal of Materials demineralized dentin matrix European Journal of Den- Science 37(22) 4733-4741. tistry 4(3) 293-297.